I. D. HARRIS
HIGH-SPEED GMAW AND LASER GMAW HYBRID WELDING OF
SCHOOL OF APPLIED SCIENCES
SCHOOL OF APPLIED SCIENCES
Academic Year 2008-2009
I. D. Harris
High-Speed GMAW and Laser GMAW Hybrid Welding of Steel Sheet
Cranfield University 2009. All rights reserved. No part of this publication may be reproduced without the written permission of the copyright owner
TABLE OF CONTENTSABSTRACT ACKNOWLEDGEMENTS LIST OF FIGURES LIST OF TABLES NOMENCLATURE ABBREVIATIONS 1.0 INTRODUCTION 1.1 Background
1.1.1 Dispelling the Myths about GMAW-P 1.1.2 The Common Myths
1.1.3 The Good News 1.2 Summary
2.0 LITERATURE REVIEW
2.1 Process Studies and Welding Productivity 2.2 Gas Metal Arc Welding
2.2.1 Gas Metal Arc Welding (GMAW) Including Pulsed GMAW (GMAW-P)
2.2.2. GMABrazing and Variable Polarity Gas Metal Arc Welding -GMAW-VP
2.2.3 STT GMAW
2.2.4 CSC and CMT GMAW
2.2.5 Tandem and Twin-Wire GMAW 2.3 Plasma Arc Welding
2.4 Hybrid Laser Arc Welding
2.5 Hybrid Laser Welding – LBW/GTAW and LBW/PAW 2.6 Hybrid Laser Welding - LBW/GMAW
2.6.1 Laser/GMAW and LBW for Galvanized Steel 2.7 Arc Power versus Laser Power
2.7.1 GMAW Melting Rate 2.7.2 GMAW Melting Efficiency 2.7.3 Laser Power and Efficiency 2.8 Diode Lasers
2.9 Fibre Lasers
2.10 Weld Bead Humping
2.11 Weld Pool Dynamics and Humping Mechanisms 2.12 Modeling
2.13 Calorimetry 2.14 Weld Sizing 2.15 Gap Weldability
2.16 A Brief Summary of Papers and Conference Presentations by the Author during the Course of This Research
2.17 Summary of the Literature Review and Work Scope in the Thesis Research
3.0 RESEARCH AIMS AND OBJECTIVES
4.0 EQUIPMENT AND MATERIALS
4.1 Welding Process and Equipment for Weld Sizing 4.2 Trumpf Programmable Focusing Optics PFO 4.3 CO2Laser System
4.3.1 High-Voltage Power Source 4.3.2 Resonator
4.3.4 Main Relay Cabinet 4.3.5 Laser Cooling System
4.4 Trumpf HAAS 4006D Neodinium Yttrium Aluminum Garnet (Nd:YAG) Laser
4.5 Workpiece Manipulation
4.5.1 Single-Axis Welding Carriage 4.5.2 CNC Worktable
4.5.3 Robotic Manipulation 4.5.4 Fixturing
4.6 Data Acquisition
4.6.1 Data Acquisition for Arc Welding 4.7 High-Speed Video (HSV)
4.8 Measurement and Analysis Tools 4.8.1 PRIMES Laser Beam Monitor
5.0 EXPERIMENTAL TECHNIQUES 5.1 Weld Acceptance Criteria
5.2 Weld Sizing Applications for Sheet Less than 3 mm 5.2.1 Welding Parameter Selection Technique 5.2.2 Weld Acceptance Criteria
5.2.3 Design of Experiments
5.3 Experimental and Theoretical Work – High-Speed GMAW-P Lap-Fillet Welding Trials
5.4 Experimental and Theoretical Work – Hybrid Welding, Laser Beam Splitting, and Toe Wetting
5.4.1 Scanning Laser Nd:YAG and Dual Spot 5.4.2 CO2Dual Beam
5.4.3 CO2Offset Beam 5.5 Calorimetry
5.6 Experimental Procedure for High-Speed Video
5.7 Accuracy and Inaccuracy of Methods, Verification, and Repeatability
6.1 Welding Parameters for Weld Sizing 6.1.1 2.4-mm Material Thickness 6.1.2 2.0-mm Material Thickness 6.1.3 1.6-mm Material Thickness
6.2 High-Speed GMAW-P for Lap-Fillet Joints 6.3 High-Speed GMAW-P for T-Joints
6.4 High-Speed Video (HSV)
6.5 Results for Hybrid LBW/GMAW-P
6.5.1 Welding Trials – GMAW with 1-kW Laser Power and PFO
6.5.2 Hybrid GMAW-P/LBW using the Trumpf HAAS 4006 Nd:YAG Laser
6.5.3 Hybrid GMAW-P/LBW with Rofin Sinar CO2Laser, Model RS-850
6.6 Results for Calorimetry 6.7 Humping Experiments 7.0 DISCUSSION 7.1 Weld Sizing 7.1.1 Deposit Area 7.1.2 Travel Angle 7.1.3 Work Angle 7.1.4 Travel Speed 7.1.5 Arc Length
7.1.6. Contact Tip to Work Distance 7.2. Energy Input and Arc Efficiency 7.3 Calorimetry
7.4 Conduction versus Convection 7.5 Wire composition and wetting 7.6 Effect of Shielding Gas 7.7 Spatter in GMAW-P
7.8 GMAW-VP and LBW/GMAW-VP 7.9 Hybrid Welding
7.9.1 Comparison of Welding Speed for GMAW-P and LBW/GMAW-P Hybrid
7.9.2 GMAW-P and LBW/GMAW-P Bead Humping – Lap Joints 7.9.3 GMAW-P and LBW/GMAW-P Bead Humping – T-Butt Joints 7.9.4. Laser Spot Size, Spacing and Power Density
7.9.5. Hybrid GMAW-P/LBW with Trumpf HAAS 4006 Nd:YAG Laser
7.9.6 Hybrid CO2Laser/GMAW-P Using the Rofin Sinar RS850 7.9.7 Laser Power versus Arc Power
7.9.8. Laser Power Distribution 7.10 Weld Bead Humping
7.10.1 Periodicity of Weld Humping in GMAW-P 7.10.2. Weld Pool Dynamics and Humping Mechanisms 7.11 High-Speed Video (HSV) Images
7.12 Impact of Results and Process Economics
9.0 RECOMMENDATIONS FOR FUTURE WORK
Arc welding is the most widely used set of joining technologies in industry today. The automotive tier supplier network and light manufacturing are significant users of arc welding, particularly gas metal arc welding (GMAW) and pulsed GMAW
(GMAW-P). For sheet metal welding the majority of welds are single pass fillet welds on T-butt, lap, or edge joints. A fundamental problem and limitation to the use of higher travel speeds in GMAW is the phenomenon of weld bead humping, a weld profile defect with a wavelike profile to the weld bead that has peaks and troughs in the longitudinal direction.
The initial hypothesis was that the humping defect can be suppressed and continuous beads deposited at much higher speeds by using a laser beam welding (LBW) in the conduction mode at the weld toes to improve bead wetting thus minimizing bead convexity which, at toe angles below 90 degrees, tends to promote the formation of the humping defect. This was investigated by a research program intended to develop an understanding of the cause of the humping defect, and included extensive use of high-speed video (HSV) to determine the root cause, from which the mechanisms were determined. The main elements of the research were as follows;
GMAW-P parameters for welding with 0T and 1T gaps (T is sheet thickness) High-speed GMAW-P with 0T gap
Hybrid LBW/GMAW-P using CO2and Nd:YAG lasers High SpeedVideo (HSV) of GMAW-P and bead humping
The hypothesis that weld pool humping can be suppressed to a travel speed (TS) well beyond that achievable with GMAW-P by directing a laser at the weld toes was demonstrated in the results achieved and their comparison to data generated for single wire GMAW-P. For the welding techniques investigated, the following maximum TS can be stated:
1. Conventional GMAW-P – typical maximum TS of 1 m/min 2. High-speed GMAW-P – typical maximum TS of 2 m/min
3. Hybrid conduction mode laser with GMAW-P – typical maximum TS of 3.3 m/min
The main conclusions are as follows:
1. Laser assisted GMAW-P allows increases in TS before humping. The
hypothesis that weld bead humping can be suppressed by using laser melting at the GMAW-P weld toes was shown by experiment to be valid.
2. HSV of GMAW-P showed a repetitive arc instability that caused the weld pool to move first forward and then backward at the moment of the instability. It also showed arc shorting leading to the end of one hump and the beginning of the next.
3. A 30-degree lead travel angle for the GMAW welding torch achieved a maximum welding speed in GMAW-P and LBW/GMAW-P welding and was beneficial in suppressing humping.
4. A work angle of 60 degrees, wire on the top edge of the top sheet, and aiming the laser at the bottom toe of the GMAW-P weld is the best configuration.
5. Aiming the wire at the top edge of the top sheet delayed the onset of bead humping to higher TS than aiming at the root.
6. Long weld pools (12:1) and no humping were achieved with a single 4 kW laser spot. Only one beam spot is required – aimed at the lower weld toe - to result in wetting.
The major benefit of this work is the increased understanding of high-speed welding and the potential to significantly increase welding productivity.
My particular thanks to my Supervisor at Cranfield University Mr. David Yapp, for interesting discussion, input, direction, and encouragement during this course of research study.
Thanks are due to the noted technical staff and colleagues at Edison Welding Institute (EWI) who have contributed in many ways. I particularly wish to thanks Mr. Michael Fallara, Mr. Brian Baughman, Mr. Matt Boring, and Ms. Joyce Hinkle of EWI for their help. I would also like to thank Professor David Farson, and Mr. HaeWoon Choi, Mr. Min Cho, and Mr. Yong Lim of The Ohio State University for their part in interesting discussion and conduction of some of the experimental work under EWI Project No. 47412GTO.
I would like to thank EWI for allowing me the opportunity to pursue this course of study, for their financial support in terms of tuition reimbursement, and for providing the extensive laboratory facilities required during a portion of the experimental program.
I would also like to thank the many member companies of EWI and the Ohio Department of Development for their mutual funding of the EWI Cooperative Research Program (CRP) which enabled the research to be conducted.
Most importantly, I wish to thank my wonderful wife Jean, and my beautiful children Avery, Paige, and Brandon for their love and support in this, as in many other
endeavors. Were it not for their forbearance and understanding of my time away from the family to complete the process, it could not have been accomplished.
LIST OF TABLES
Table 2.1. Lasers and Optics Used for Welding
Table 6.1. Measurement of Fillet Weld Leg Lengths, Area, and Toe Angle Against Lower Sheet
Table 6.2. Nd:YAG Trials with PFO
Table 6.3. 4-kW Nd:YAG/GMAW Hybrid Trials With Split Optics – Lap Joints
Table 6.4. Parameters for CO2Laser/GMAW-P Hybrid BOP, Lap and T-Butt Joints
Table 6.5. Weld Leg Length, Weld Area and Weld Toe Angles
Table 6.6 Results for GMAW-P Calorimetry and Plot of Results
Table 6.7 Weld Type and Welding Parameters for HSV Trials
Table 6.8 Results for Hybrid LBW/GMAW-P Calorimetry and Plot of Results
Table 7.1. Calculated Weld Deposit Areas for all Three Material Thicknesses Using Preferred WFS and TS
Table 7.2. Weld Deposit Area Measurements Made with ImagePro™Software of All Three Material Thicknesses Welded Using Preferred WFS and TS
Table 7.3. Causes and Remedies of Undercut
Table 7.4. Methods of Reducing Various Welding Process Defects in GMAW Including the Humping Defect
Table 7.5 Oxidation Potential of Various Metals and Oxides and their Stability (AWS, 2004)
LIST OF FIGURES
Figure 2.1 Gas Metal Arc Welding Process
Figure 2.2 Features of GMA-Brazing
Figure 2.3 Nominal Comparison of Penetration and Wire Melting Rate for GMAW-DCEP and GMAW-DCEN
Figure 2.4 Miller Jetline CSC Gun Showing Dual-Wire Drive Motors
Figure 2.5 Fronius CMT Gun with Integrated Dual-Wire Feed Motors
Figure 2.6 Twin-Wire and Tandem GMAW
Figure 2.7 Tandem GMAW Torch with Dual Contact Tips
Figure 2.8 Typical Arrangement of a Tandem GMAW Welding Torch Head
Figure 2.9 Schematic of LBW/GMAW Operation
Figure 2.10 Plasma Welding Torch With Cold Wire Feed
Figure 2.11 Fronius Hybrid LBW/GMAW Welding Head for Robotic Applications
Figure 2.12 Schematic of LBW/GMAW Operation and Features of Hybrid Welding
Figure 2.13 Twin-Spot (Dual-Beam) Optics for Nd:YAG Lasers (Goebels et al., 2003)
Figure 2.14 Representation of the Forces on an Electrode Drop in GMAW (Norrish and Richardson, 1988)
Figure 2.15 Changes in the Forces on an Electrode Drop as the Welding Current Increases (Pintard, 1966)
Figure 2.16 Laser Spot Diameter versus Laser Power Required for Stabilization
Figure 2.17 Laser Melting Efficiency in Mild Steel (Ream, 2004)
Figure 2.18 Classic Continuous Bead Humping in GMAW BOP (top)
Figure 2.19 Weld Appearance for Classic Discontinuous Bead Humping in GMAW
Figure 2.20 Weld Pool Fluid Flow as Observed and Proposed by Bradstreet for High-Speed GMAW
Figure 2.21 Contact Line Behaviour – (Schiaffino and Sonin, 1997 )
Figure 2.22 Rearward Weld Metal Fluid Flow Including the Effect of Arc Pressure and Wire Droplet Addition (Kim and Na, 1995)
Figure 2.23 Flow 3-D Simulation of GMAW-P Droplet Crossing the Arc to the Weld Pool (Cho and Farson, 2007)
Figure 2.24 BOP Bead Humping Simulation at 2.5 m/min TS and 25 m/min WFS (Cho and Farson, 2007)
Figure 2.25 Hybrid Welding Process Concept for GMA Spot Welding
Figure 2.26 Arc Melting Efficiency (DuPont and Marder, 1995).
Figure 2.27 The Principle of Self-Fixturing of the Weld Components
Figure 2.28 Tab-and-slot Assembly Procedure (Caterpillar)
Figure 4.1 Standard Fixture for Lap-Fillet Joints
Figure 4.2. Welding Power Supply and Wire Feeder (left), Data Acquisition System (Right) used for Gap Weldability Testing
Figure 4.3. Assembled Variable Joint Gap Weldability Fixture
Figure 4.4 Side View of Joint Setup to Determine Critical Support Location
Figure 4.5 Gap Geometry for DOE Trials
Figure 4.6 Equipment Setup for High-Speed GMAW-P Welding Trials to Establish Humping Limits
Figure 4.7 Principle for Rapid Beam Manipulation in the PFO Scanner
Figure 4.8 The Trumpf Programmable Focusing Optics Device
Figure 4.9 CNC Nd:YAG/GMAW-P Setup for PFO Evaluation, Including HSV, DAQ, and LASEdit Laser Programmer/Controller
Figure 4.10 Rofin Sinar 850 CO2Laser Was Used for Single- and Dual-Beam LBW/GMAW-P Hybrid Welding
Figure 4.11 Waveguide for Beam Delivery to the GMF Robot
Figure 4.12 Single-Spot Laser Mirror System for Robotic CO2Laser Welding
Figure 4.13 Rear Face of Split (wire EDM) Copper Mirror for Dual-Spot Experiments with a CO2Laser
Figure 4.14 GMF Robotics Karel L-100 Robot Controller
Figure 4.15 Laser Spot Alignment Using Low Power Visible Red He-Ne Laser
Figure 4.16 Console for Laser Parameter Selection
Figure 4.17 Trumpf Haas HL 4006 4-kW Continuous-Wave Nd:YAG
Figure 4.18 Motoman SK16 Robot with Fibre-Delivered Nd:YAG Laser and ESAB GMAW-P Equipment Setup on a Lap Joint
Figure 4.19 GMAW-P Waveform from Arc Impact DAQ at 10-kHz Sampling Frequency
Figure 4.20 Kodak Ektapro HS HSV Camera Setup for Viewing the Weld Pool Perpendicular to the Welding Direction
Figure 4.21 Cover Lens and IR Band-Pass Filter Attached to the Camera Lens
Figure 4.22 Digital Download Interface for Triggering and Capturing HSV Data
Figure 4.23 Typical Screen Image and Frame Data Using the Kodak Ektapro HS System
Figure 4.24 Phantom HSV Camera With Filter Mount Between the Camera and Lens Assembly
Figure 4.25 Primes™Beam Power Analysis System Setup to Measure Distributed Power in Dual-Beam Nd:YAG Laser
Figure 4.26 WISC Laser Profilometer
Figure 4.27 Equipment Used for Calorimetry Experiments
Figure 5.1 Gap Geometry for DOE Trials
Figure 5.2. Sample of Completeness of Fusion Rating used by Richardson
Figure 5.3. Illustration of a “Skip”, or Incomplete Fusion, Encountered During Welding Denoting the End of the Acceptable Weld
Figure 5.4 Typical Bead Humping Defect in a Lap-Fillet Weld
Figure 5.5 100-W Dual-Beam Nd:YAG Laser Burn Pattern on Thermographic Paper to Illustrate TEM 01 Laser Mode
Figure 5.6 Fibre-Delivered Nd:YAG Laser and ESAB GMAW-P Equipment Setup on a Lap Joint for Single- and Dual-Spot Welding Trials
Figure 5.7 100-W Dual Beam Nd:YAG Laser Burn Pattern on Thermographic Paper to Illustrate TEM 01 Laser Mode
Figure 5.8 Fibre-Delivered Nd:YAG Laser and ESAB GMAW-P Equipment Setup on a Lap Joint for Single- and Dual-Spot Welding Trials
Figure 5.9 CO2Laser Burn Pattern on Perspex for Dual Beam in TEM 01 Mode
Figure 5.10 Control Block Diagram of the Calorimetry Experiments
Figure 5.11 Calibration Image for HSV Using a Millimeter Scale
Figure 6.1. WFS versus Voltage Relationship for Maintaining a Constant 3.2-mm Arc Length Using GMAW-P with a 19-mm CTWD and a 1.2-mm-Diameter ER70S-3 Electrode
Figure 6.2 SWAT Results Showing the Visually Acceptable Weld Area Curve for 2.4-mm Mild Steel with a 0T Joint Gap
Figure 6.3. SWAT Results Showing the Destructively Tested Acceptable Weld Area Curve for 2.4-mm Mild Steel with a 0T Joint Gap
Figure 6.4. Macrosection Map for 2.4-mm Lap Joints with a 0T Joint Gap
Figure 6.5. SWAT Results Showing the Acceptable Weld Area Curve for 2.4-mm Mild Steel with a 1T Joint Gap.
Figure 6.6. Macrosection Map for 2.4-mm Lap Joints with a 1T Joint Gap
Figure 6.7. SWAT Results Showing Acceptable Weld Area Curve for 2.0-mm Mild Steel Lap joints with a 0T Joint Gap
Figure 6.8. Macrosection Map for 2.0-mm Sheet Lap Joints with 0T gap
Figure 6.9. SWAT Results Showing Acceptable Weld Area Curve for 2.0-mm Mild Steel Lap Joints with a 1T Joint Gap
Figure 6.10. Macrosection Map for 2.0-mm Lap Joints with a 1T Joint Gap
Figure 6.11. SWAT Results Showing Acceptable Weld Area Curve for 1.6-mm Mild Steel Lap joints with a 0T Joint Gap
Figure 6.12. Macrosection Map for 1.6-mm Lap Joints with a 0T Joint Gap made using a 1.2-mm-Diameter ER70S-3 Electrode Wire
Figure 6.13. SWAT Results Showing Acceptable Weld Area Curve for 1.6-mm Mild Steel Lap Joints With a 1T Joint Gap
Figure 6.14. Macrosection Map for 1.6-mm Lap Joint with a 1T Joint Gap Made Using a 1.2-mm-Diameter ER70-S3 Electrode Wire
Figure 6.15. Developed Weld Area for the 2.4-mm Mild Steel Sheet Applied to a 0T Joint Gap (left) and 1T Joint Gap (Right)
Figure 6.16. Developed Weld Area for the 2.0-mm Mild Steel Sheet Applied to a 0T Joint Gap (left) and 1T Joint Gap (Right)
Figure 6.17. Developed Weld Area for the 1.6-mm Mild Steel Sheet Applied to a 0T Joint Gap (Left) and 1T Joint Gap (Right)
Figure 6.18. Macrosections of Fillet Welds on T-Butt Joints for the Three Material Thicknesses Studied.
Figure 6.19. Continuous Humping Defect Generated at a 1T Gap on a Joint at a ‘High’ Travel Speed of 1.0 m/min.
Figure 6.20. 2.4-mm Sheet, WFS 12.7 m/min, TS 1.0 m/min, 1T Gap
Figure 6.21. Further Examples of Humped Bead Profiles for 2.4- and 2.0-mm Sheet
Figure 6.22. Bead Humping Limit for High-Speed GMAW-P versus ‘Conventional’ GMAW-P
Figure 6.23. Bead Humping Limit for High-Speed GMAW-P versus ‘Conventional’ GMAW-P
Figure 6.24. Bead Humping Limit for High-Speed GMAW-P versus ‘Conventional’ GMAW-P for Lap-Fillet Joints in 1.6-mm Sheet
Figure 6.25. Weld Appearance Map for 2.4-mm Sheet Lap-Fillet Joints with 0T Gap
Figure 6.26. Bead Humping Limit and Acceptable Weld Area for High-Speed GMAW-P versus ‘Conventional’ GMAW-P for 2.4-mm Sheet
Figure 6.27. Weld Appearance Map for 2.0-mm Sheet Lap-Fillet Joints with 0T Gap
Figure 6.28. Bead Humping Limit and Acceptable Weld Area for High-Speed GMAW-P versus ‘Conventional’ GMAW-P
Figure 6.29 Weld Appearance Map for 1.6-mm Sheet Lap-Fillet Joints with 0T Gap
Figure 6.30. Bead Humping Limit and Acceptable Weld Area for High-Speed GMAW-P versus ‘Conventional’ GMAW-P
Figure 6.31. Macrosections Through Bead Humps at the Limits of Travel Speed for Each Material Thickness
Figure 6.32. Weld Appearance Map for Fillet Welds on T-Butt Joints Using 2.4-mm Sheet
Figure 6.33. Weld Appearance Map for Fillet Welds on T-Butt Joints Using 2.0-mm Sheet
Figure 6.34. Weld Appearance Map for Fillet Welds on T-Butt Joints Using 1.6-mm Sheet
Figure 6.35. HSV Images (GMAWP186- GMAWP214) for GMAW-P
Figure 6.36. Initial PFO Trials With 1-kW Nd:YAG Laser
Figure 6.37. Spot and Scanned Nd:YAG Laser Profiles in BOP Form
Figure 6.38. HSV of GMAW-P Metal Transfer and 1-kW PFO Laser Spot
Figure 6.39. Nd:YAG Spot and Corresponding LBW/GMAW-P BOP Weld
Figure 6.40. 2-mm Scanned Nd:YAG and Corresponding LBW/GMAW-P BOP
Figure 6.41. 4-mm Scanned Nd:YAG and Corresponding LBW/GMAW-P BOP Weld
Figure 6.42. Classic Bead Humping Suppressed with 1-kW Nd:YAG Laser Energy (WFS/TS of 5 - BOP weld) at 2.0-m/min Travel Speed
Figure 6.43. Profile for 4-kW Nd:YAG Laser with a Single Beam at Focus with 200-mm Optics
Figure 6.44. Beam Profile for 4-kW Nd:YAG Laser with Dual-Beam Using 200-mm Focusing Optics (Profile of One Beam is Shown)
Figure 6.45. 100-W Dual-Beam Nd:YAG Laser Burn Pattern on Thermographic Paper to Illustrate TEM 01 Laser Mode
Figure 6.46. Single-Beam Laser Offset to GMAW Weld Toe to Increase Toe Wetting Using an Nd:YAG Laser
Figure 6.47. GMAW-P Fillet Weld on a Lap Joint
Figure 6.48. Hybrid Nd:YAG/GMAW Fillet Weld on a Lap Joint
Figure 6.49. 42-mm-Long Weld Pool with 3-mm Bead Width (14:1) Using Single-Spot 4-kW Nd:YAG/GMAW-P Hybrid Welding on a Lap Joint
Figure 6.50. Bead Appearance for Dual-Spot Nd:YAG Hybrid Weld made at 3.3 m/min on a Lap-Fillet Joint on 2.4-mm Sheet
Figure 6.51. Macrosection for Dual-Spot Nd:YAG Hybrid Weld Made at 3.3 m/min on 2.4-mm Sheet
Figure 6.52. Macrosection for Dual-Spot Nd:YAG Hybrid Weld Made at 4.0 m/min on 2.4-mm Sheet
Figure 6.53. Profile of 6-kW CO2Laser Beam at Focus with 254-mm Optics
Figure 6.54. CO2Laser Burn Pattern on Perspex for Dual Beam in TEM 01 Mode Using 3.2, 6.4 and 9.5-mm Dual Spot Spacing
Figure 6.55. Weld Appearance Map for Hybrid CO2LBW/GMAW-P BOP Welds on 2.4-mm Sheet
Figure 6.56. BOP Weld Made Using Single-Spot Laser at 3.3-kW and 2.5-m/min Travel Speed on 2.4-mm Sheet
Figure 6.57. BOP Weld Made Using Single Spot Laser at 3.3-kW and 3.0-m/min Travel Speed on 2.4-mm Sheet
Figure 6.58. Weld Appearance Map for Hybrid CO2LBW/GMAW-P Lap-Fillet Welds on 2.4- and 2.0-mm Steel Sheet
Figure 6.59. Bead Appearance for a Lap-Fillet Joint made using Single-Spot CO2 LBW/GMAW-P Hybrid Welding With 3.25-kW Laser Power at 4-m/min Travel Speed on 2-mm Sheet
Figure 6.60. Macrosection for Single-Spot CO2LBW/GMAW-P Hybrid Weld Made at 4 m/min on 2-mm Sheet
Figure 6.61. Weld Appearance Map for Fillet Welds on 2.4-mm Steel Sheet Using CO2LBW/GMAW-P Hybrid Welding
Figure 6.62. Bead Appearance for a T-Butt Joint Made Using Single-Spot CO2 LBW/GMAW-P Hybrid Welding at 3 m/min on 2-mm Sheet
Figure 6.63. Macrosection (on Left – Tack on Right) for a Single-Spot CO2
LBW/GMAW-P Hybrid Weld Made With 3.5-kW Laser Power at 3.0 m/min on 2-mm Sheet
Figure 6.64. Macrosection for a Dual-Spot CO2LBW/GMAW-P Hybrid Weld Made at 1.75 m/min on 2-mm Sheet
Figure 6.65. Plan View of GMAW-P Weld Pool Cavity for Specimen 72805a WFS 15.2 m/min, TS 2.5 m/min, 225 A, 37 V, 19-mm CTWD
Figure 6.66. Side View of GMAW-P BOP Humping for Specimen 72805a WFS 15.2 m/min, TS 2.5 m/min, 225 A, 37 V, 19-mm CTWD
Figure 6.67. Plan View of GMAW-P BOP Humping for Specimen 72805a WFS 15.2 m/min, TS 2.5 m/min, 225 A, 37 V, 19-mm CTWD
Figure 6.68. HSV Sequence of Bead Humping and Solidification
Figure 6.69. Plan View of GMAW-P BOP Humping for Specimen 72805 WFS 15.2 m/min, TS 2.5 m/min, 225 A, 28 V, 19-mm CTWD
Figure 6.70. Side View of GMAW-P BOP Humping for Specimen 72805 WFS 15.2 m/min, TS 2.5 m/min, 225 A, 37 V, 19-mm CTWD
Figure 6.71. HSV Sequence for GMAW-P Bead Humping
Figure 6.72. Plan View of GMAW-P BOP Humping and Weld Pool Cavity for Specimen 72805c WFS 15.2 m/min, TS 2.5 m/min, 225 A, 31 V, 19-mm CTWD
Figure 6.73. Side View of GMAW-P BOP Humping and Weld Pool Cavity for Specimen 72805c WFS 15.2 m/min, TS 2.5 m/min, 225 A, 31 V, 19-mm CTWD
Figure 6.74. HSV Sequence for GMAW-P Weld 72805c
Figure 6.75. Plan View of GMAW-P BOP Humping and Weld Pool Cavity for Specimen 72905a WFS 15.2 m/min, TS 2.5 m/min, 225 A, 33 V, 16-mm CTWD
Figure 6.76. Side View of GMAW-P BOP Humping for Specimen 72905a WFS 15.2 m/min, TS 2.5 m/min, 225 A, 33 V, 16-mm CTWD
Figure 6.77. Plan View of GMAW-P BOP Humping and Weld Pool Cavity for Specimen 72905-3 WFS 15.2 m/min, TS 2.5 m/min, 225 A, 35 V, 16-mm CTWD
Figure 6.78. Side View of GMAW-P BOP Humping and Weld Pool Cavity for Specimen 72905-3 WFS 15.2 m/min, TS 2.5 m/min, 225 A, 35 V, 16-mm CTWD
Figure 6.79. Plan View of GMAW-P BOP Humping (Upper Bead) and Weld Pool Cavity for Specimen 80205a WFS 15.2 m/min, TS 2.5 m/min, 225 A, 34 V, 19-mm CTWD
Figure 6.80. Side View GMAW-P BOP Humping and Weld Pool Cavity for Specimen 80205a WFS 15.2 m/min, TS 2.5 m/min, 225 A, 34 V, 19-mm CTWD
Figure 6.81. Plan View of GMAW-P BOP Humping and Weld Pool Cavity for Specimen 80205b WFS 15.2 m/min, TS 2.5 m/min, 225 A, 34 V, 19-mm CTWD WFS 15.2 m/min, TS 2.5 m/min, 225 A, 34 V, 19-19-mm CTWD
Figure 6.82. Side View of GMAW-P BOP Humping and Weld pool Cavity for Specimen 80205b WFS 15.2 m/min, TS 2.5 m/min, 225 A, 34 V, 19-mm CTWD
Figure 6.83. Side View GMAW-P BOP Humping for Specimen 80205b WFS 15.2 m/min, TS 2.5 m/min, 225 A, 34 V, 19-mm CTWD
Figure 6.84. Plan View of GMAW-P Fillet Weld Humping in a Lap Joint for Specimen 80305a WFS 15.2 m/min, TS 3.0.5 m/min, 225 A, 34 V, 16-mm CTWD
Figure 6.85. Side View of GMAW-P Fillet Weld Humping in a Lap Joint for Specimen 80305a WFS 15.2 m/min, TS 3.0 m/min, 225 A, 34 V, 16-mm CTWD
Figure 6.86. Plan View of LBW/GMAW-P Fillet Weld Humping in a Lap Joint for Specimen 80305b with Wire Offset too Much onto the Top Sheet WFS 15.2 m/min, TS 3.0 m/min, 225 A, 34 V, 16-mm CTWD
Figure 6.87. Side View of LBW/GMAW-P Fillet Weld Humping in a Lap Joint for Specimen 80305b with Wire Offset too Much onto the Top Sheet WFS 15.2 m/min, TS 3.0 m/min, 225 A, 34 V, 16-mm CTWD
Figure 6.88. HSV Stills of a Lap Fillet Weld Viewed ‘Head-On’
Figure 6.89. Plan View of GMAW-P BOP Humping for Specimen 82405-5 WFS 15.2 m/min, TS 3.0 m/min, 225 A, 34 V, 16-mm CTWD
Figure 6.90. Side View of GMAW-P BOP Humping for Specimen 82405-5 WFS 15.2 m/min, TS 3.0 m/min, 225 A, 34 V, 16-mm CTWD
Figure 6.91 HSV Showing Short Circuiting of the Wire to the Weld Pool in BOP Specimen 082405-4 at the Point when a New Hump is Created
Figure 6.92. HSV Still Sequence Showing Expulsion and Weld Pool Motion
Figure 6.93. HSV Still Sequence Showing Expulsion and Weld Pool Motion
Figure 6.94. HSV Still Sequence Showing Expulsion and Weld Pool Motion
Figure 6.95. Plan View of GMAW-P BOP Humping for Specimen 82405-8 WFS 15.2 m/min, TS 3.0 m/min, 225 A, 34 V, 16-mm CTWD
Figure 6.96. Side View of GMAW-P BOP Humping for Specimen 82405-8 WFS 15.2 m/min, TS 3.0 m/min, 225 A, 34 V, 16-mm CTWD
Figure 6.97. HSV Images Showing Weld Pool Motion through Movement of the ‘White’ Silicate Slag Islands
Figure 6.98. Three Images in Sequence (082405-8 HSV File) Showing Weld Pool Motion First Forward then Backward
Figure 6.99. Two Images Five Frames Apart (082405-8 HSV File) Showing Repetition of Weld Pool Forward Motion Every Ten Frames
Figure 6.100. Plan View of GMAW-P Fillet Weld Humping in a Lap Joint, Specimen 83005-1
Figure 6.101 HSV Showing Short Circuiting of the Wire to the Weld Pool and Arc Re-Ignition in Lap Fillet Specimen 083005-b
Figure 6.102. Plan View of GMAW-P Fillet Weld Humping in a Lap Joint, Specimen 83005-2
Figure 7.1. Electrode Locating Error
Figure 7.2 Plan View of GMAW-P Fillet Weld Discontinuous Humping in a Lap Joint, Specimen 83005-2 Resulting from Wire Mislocation onto the Top Sheet
Figure 7.3. CTWD Changes
Figure 7.4. 40-mm-Long Weld Pool with 3-mm Bead Width (14:1) using Single-Spot 4-kW Nd:YAG/GMAW Hybrid on a Lap Joint
Figure 7.5. Wetting of the Weld Toe Using a Single Laser Spot (Seen at Left of Righthand Weld Bead)
Figure 7.6 Onset of Bead Humping for Lap Joints Made Using GMAW-P
Figure 7.7 WFS/TS Versus TS Showing That Smaller Welds Can be Made at Higher TS
Figure 7.8 Trends for Weld Size Ratio (WFS/TS) versus TS for Lap Joints Made with Conventional GMAW-P, High-Speed GMAW-P, and
Figure 7.9 Trends for Weld Size Ratio versus TS for Conventional GMAW-P, High-Speed GMAW-P, and LBW/GMAW-P Hybrid Welding in T-Butt Joints
Figure 7.10 Plan View - Arrangement of Laser beam Spots (Round) Relative to the Arc Weld Pool (Ellipse) to Achieve Maximum Weld Toe Wetting and Spreading
Figure 7.11 Cross-Sectional view - Arrangement of Laser beam Spots (Small Ellipses) Relative to the Arc Weld Pool (Larger Ellipse) at Left, to Achieve Maximum Weld Toe Wetting and Spreading, at Right
Figure 7.12 Plan View - Size and Arrangement of Laser beam Spots (Round) Relative to the Arc Weld Pool (Ellipse) Resulting in Minimum Weld Toe Wetting and Spreading
Figure 7.13 Cross-Sectional View - Size and Arrangement of Laser beam Spots (Small Eliptical Spot) Relative to the Arc Weld Pool (Ellipse) at Left, Resulting in Minimum Weld Toe Wetting and Spreading at Right
Figure 7.14 Plan View - Arrangement of Laser Beam Spots (Round) Relative to the Arc Weld Pool (Ellipse) Resulting in Insufficient Melting by the Laser and Thus No GMAW-P Toe Wetting and Spreading
Figure 7.15 Cross-Sectional View - Arrangement of Laser beam Spots (Small Ellipses) Relative to the Arc Weld Pool (Ellipse) at Left, Resulting in Insufficient Melting by the Laser and Thus No GMAW-P Toe Wetting and Spreading, at Right
Figure 7.16 36-mm-Long Weld Pool with 3-mm Bead Width (12:1) Using Single-Spot 4-kW Nd:YAG/GMAW-P Hybrid on a Lap Joint
Figure 7.17 Side View of GMAW-P BOP Humping for 2.4-mm Sheet Specimen 72805
Figure 7.18 Side View of GMAW-P BOP Humping in 1.6-mm Sheet Metal for Specimen 80205b
Figure 7.19 Repetitive Forward and Backward Motion of the GMAW-P Weld Pool Within 2 frames (Images 309, 31, and 310) at 250 fps
Figure 7.20 HSV Still Sequence Showing Weld Wire Expulsion and Weld Pool Motion
Figure 7.21 HSV Still Showing Weld Wire Expulsion and Weld Pool Motion
Figure 7.22 HSV Still Showing Weld Wire Expulsion and Weld Pool Motion
Figure 7.23 HSV Showing Short Circuiting of the Wire to the Weld Pool in BOP Specimen 082405-4
Figure 7.24 HSV Showing Short Circuiting of the Wire to the Weld Pool and ArcRe-Ignition in Lap Fillet Specimen 083005-1
Figure 7.25 Classic Bead Humping (Top Bead) for GMAW-P Suppressed with 1-kW Nd:YAG Laser Energy (Middle and Bottom) (WFS/TS of 5 - BOP Weld) at 2.0-m/min TS
Figure 7.26 Distribution of Welding Consumable Use by Industry (Pekkari, 2004)
Figure 7.27 Energy Usage and Efficiency for an Array of Commonly Used Welding Processes (Pekkari, 2004)
Figure 9.1 Extrapolation of TS and WFS for Higher Productivity Using Hybrid LBW/TGMAW-P
fps feet per second
kg/h kilograms per hour
kJ/mm kilojoules per millimeter l/min litres per minute
m/min metres per minute
mm/min millimetres per minute mm3/kJ millimeters cubed/kilojoules
ppm parts per million
Mtonnes Millions of tonnes W/m2 Watts per square metre W/mm2 Watts per square millimetre
A Amperes (welding current)
AC Alternating current
AHSS Advanced high-strength steels
AIP Average instantaneous power
ANOVA Analysis of variance
AWS American Welding Society
BIW Body in white
BOP Bead on plate
CMT Cold metal transfer
CRP Cooperative Research Program
CAD Computer-aided design
CAM Computer-aided manufacturing
CMOS Complementary metal oxide semiconductor
CNC Computer numerical control
CSC Controlled short circuit CTWD Contact tip to work distance
CV Constant voltage
DAQ Data acquisition
DCEN Direct current electrode negative
DOE Design of experiments
DC Direct current
DCEP Direct current electrode positive
EDM Electro discharge machining
EP/EN Electrode positive/electrode negative
EWI Edison Welding Institute
FEM Finite-element modeling
FGD Flue gas desulphurization
GMAW Gas metal arc welding
GMAW-VP Variable-polarity GMAW
GMAW-P Pulsed-current GMAW
GMAW-SC Short-circuit GMAW
GMAW-MP Mechanically pulsed GMAW GTAW Gas tungsten arc welding
HLAW Hybrid laser arc welding
KB-DOE Knowledge-based design of experiments LAAW Laser-assisted arc welding
LANL Lawrence Livermore National Lab
LED Light emitting diode
LBW Laser beam welding
Nd:YAG Neodymium-doped yttrium aluminum garnet
NG Narrow groove
ODOD Ohio Department of Development
OSU The Ohio State University
PC Personal computer
PAW Plasma arc welding
PFO Programmable focusing optics
PMCS Power measurement calorimetric system
PSNS Puget Sound Naval Shipyard
ROI Return on investment
RSW Resistance spot welding
RSM Response surface methodology
RMS Root mean square
RE-GMAW Rotating electrode GMAW RLT-GMAW Rotating lead tandem GMAW
SC Short circuit
SEC Seebeck envelope calorimeter STT Surface tension transfer SWAT Sloping weld area testing SUV Sport utility vehicle
TS Travel speed
TGMAW Tandem GMAW
TIME Transferred Ionized Molten Energy
TTA Through the arc
VOF Volume of fluid
V Volts (arc voltage)
Arc welding represents the most widely applied set of joining process, and within this suite of processes gas metal arc welding (GMAW) is the most widely used,
accounting for 74% of the Western European consumables market, 59% of the market in the USA, and 55% in Japan, in 2002 (Pekkari, 2005). The reason for this is that the process combines the elements of low capital and running cost, simplicity and
flexibility in application and can be used to weld a wide range of metals and alloys. The GMAW process can be used by hand (semi-automatic, rather than manual since the wire feed is mechanized), with simple linear or hard automation, or most flexible of all, in conjunction with modern six-axis robots within flexible automation work cells. The latter is of most interest, especially in today’s increasingly globally competitive marketplace since it provides the lowest labor cost and highest productivity.
While the use of Al alloys and other metals is increasing, by far the most widely used metal is steel, in a wide array of strengths and thicknesses. In 2003 about 26.4 Mtonnes of Al were produced compared to 855.0 Mtonnes of steel (Pekkari, 2004). To counter the higher use of Al in the automotive industry, the steel industry has introduced advanced high-strength steels (AHSS) in the body and other parts of the structure. In the automotive, shipbuilding, and other industries the use of steel is very high and the trend is increasingly to thinner and higher strength grades. This is reflected in the welding market, wherein the automotive, automotive supplier and general (light) industry account for 60% of the market. Sheet steels and thin plate represent the majority of material consumed and this trend results in the fact that most welds, even in a heavy construction area like shipbuilding are made with a single weld pass. Thus, high productivity welding of joints that can be completed in a single pass is the most prevalent and any process that can increase the productivity of joint completion is of great interest.
While there are several joint types, they can be reduced to only a few basic types, about 80% being fillet welds in either T-butt joints, or lap joints. The other major type is groove welds in butt joints, and makes up the majority of the other 20%. Therefore, it is clear that higher productivity of fillet welding will have the highest impact on overall productivity for single-pass welds.
A fundamental problem and limitation to the use of higher travel speeds in GMAW is the phenomenon of weld bead humping, a weld profile defect with a wavelike profile to the weld bead that has peaks and troughs in the longitudinal direction. In current practice the best way to avoid this is simply to limit the travel speed to one below the threshold for humping. These problems are exacerbated by thinner sheet often associated with the increased use of AHSS.
The main drivers for increased welding productivity are economic and are associated with the need to reduce weight in the vehicle for increased performance and/or fuel economy. A substantial part of the weight reduction is achieved by increased use of thinner gauge AHSS.
Weight Reduction - Higher performance, improved economy, and increasing optional equipment create continued pressure on structural and body
components. Thinner, higher strength steels, Al, Mg, and plastics are all being introduced and/or substituted to achieve weight targets. Even the larger sport utility vehicle (SUV) and truck categories face this challenge.
Welding Solutions for AHSS - The biggest change in automotive materials since the broad application of galvanized steel is the introduction of AHSS, which contain sufficient carbon to produce less ductile weld regions (among other challenging issues). In order to achieve acceptable fatigue and impact strengths with these new steels, advances in resistance spot welding (RSW), GMAW, and laser beam welding (LBW) will be required.
High-speed welding of thin sheet, new products, cost pressures, and quality concerns are all driving demand for higher welding speeds on thinner metal components. Higher speed welding processes, such as laser, laser-hybrid, pulsed GMAW (GMAW-P), and plasma arc welding (PAW) are receiving greater attention. Automotive and light manufacturing challenges almost always involve repetitive, automated, welding processes that demand precision motion and accurate control.
In addition to productivity, cost goes hand in hand, and should be considered in terms of capital cost, running cost, and return on investment (ROI). Many capital
investments choices are made on the basis of ROI, and the acceptable period for ROI varies from several months to a year in many cases.
The factors relating to the subject matter at hand can be summarized as follows: Almost all welds are single pass
Acceptable quality and productivity are the key items
Weld sizing is not well defined, especially for welding of sheet metal. Weld sizing refers to the preferred weld cross-sectional area and/or fillet leg length. Most data is based on single torch GMAW in either short-circuit (SC) mode or
using GMAW with direct current (DC) or GMAW-P
Use of computer-aided design (CAD) and computer-aided manufacturing (CAM) and computer numerical control (CNC) bending to increase part accuracy and reduce fit-up problems
Use of CNC laser cutting and CNC punch presses to produce accurate parts and make part changes to improve fit-up
Welding is expected to cope with the tolerances – and with tolerance stack-up that may lead to significant gaps
In contrast to the point above, a target of zero gap can be aimed for with accurate forming and fixturing and increased use of CAD/CAM – this will help maximize welding productivity, and minimize production costs Sheet metal fabrication is very important in the automotive and light
High-strength steels and down-gauging to thinner, lighter weight material – issue of Al versus steel performance and cost
Cost and performance issues for fabrication of thinner gauge, lighter weight vehicles, and structures of many kinds, even in the shipbuilding arena
In a scenario of continuous improvement and cost reduction, welding productivity increases through robotics and automation have and will continue to be achieved. The development of newer welding techniques and processes is often aimed at higher productivity through the use of higher welding speeds and thus deposition rates. A big impediment to welding productivity is the tendency to over-weld small fillet welds in thin plate and sheet products. Over-welding results in higher welding costs, including additional welding power, electrode wire, higher distortion (and distortion correction costs), and lost productivity.
Prior operations in the fabrication sequence, such as cutting and forming, typically lead to gaps in weld joints. Flexible and fairly gap tolerant welding processes such as GMAW have traditionally been expected to cope with these gaps in the welding operation. However, gaps can severely limit productivity by limiting the TS that can be used. Poor fixturing used during welding can also be a cause of poor part fit-up. The wire fed arc welding processes are most tolerant to gaps as filler material can be deposited to bridge the joint gap.
The use of variable-polarity GMAW (GMAW-VP) has been limited because the power sources are current limited to only 200-300 A. This, in turn, limits the welding speed and has made the equipment of less commercial interest compared to the much greater flexibility and power capabilities of 500-A inverter power sources for GMAW and GMAW-P. Higher power inverter GMAW-P power sources with electronic control of ‘arc re-ignition’ allows short arc lengths and low arc voltages to be used to control bead width.
Emerging technical capabilities of mechanically pulsed GMAW (GMAW-MP) equipment such as the Controlled Short Circuit (CSC) from Jetline/Miller and Cold Metal Transfer (CMT) from Fronius provide exceptional control of the welding arc for GMAW in SC mode by employing advancing and retracting wire drive. While this is of significant interest for light manufacturing and aerospace, the equipment is also current limited by the nature of the use of the SC current regime, and the
equipment is thus not suited to high welding speeds in the 2-4-m/min range of interest here.
Two processes that are relatively new are tandem GMAW (TGMAW) and
laser/hybrid GMAW. Both offer the flexibility to apply to plate products and thicker sheet products, with limits generally accepted to be around 1.6-mm thickness at the lower end.
The economics of the welding operation are usually fairly complex, but comparing processes on a use and cost of energy per meter of weld is a reasonable way to present this, especially when energy costs are increasingly high. Such a comparison (Pekkari, 2004) for full-penetration welding of 4-mm-thick carbon steel butt joints, shows the kJ/m for Nd:YAG, lamp-pumped lasers to be almost as high as for GMAW, 1650 kJ/m compared with 1800 kJ/m, respectively. This is quite surprising initially, but the efficiency of such a laser is only 1-2 %, compared to an efficiency of 10-15% for a CO2laser. Economically, it is fairly clear that CO2/GMAW hybrid welding is more energy efficient than Nd:YAG/GMAW hybrid welding, and the capital equipment cost of the CO2laser is considerably cheaper than that of the Nd:YAG laser. An
advantage of Nd:YAG lasers is that they are fibre deliverable and thus more suitable for robotic deployment compared with CO2lasers. TGMAW, with similar
productivity for some applications is an attractive proposition since the capital cost is significantly lower compared to laser systems.
In aerospace the buy to fly cost is of increasingly critical importance and the next level of performance is sought in the arena of hypersonic vehicles. For various performance and strength to weight requirements, the increasing use of lightweight Ti and Ni alloy structures is being actively researched by the author. Material thickness ranges of 0.5 to 1.75 mm are typical in these cases and high-speed GMAW-P, LBW and LBW/GMAW-P are the main contenders for process selection and research.
The concepts and results of the research presented in this thesis can also be used for Ti and Ni alloys, as well as steel, stainless steel, and Al alloys. An example from the author’s experience based on process selection for Ni-based alloys comes from a project funded by a major welding equipment manufacturer to highlight the
productivity benefits of their new electronically controlled SC GMAW power source (Harris, 1998). The application area of interest was the flue gas desulphurization (FGD) market for power generation market sector. FGD involves scrubbing sulphur compounds from the flue gas before it is discharged and a leading technique is to ‘wallpaper’ the steel flue stack with a lining of a Ni-based alloy, typically C-276. The context of the research was to compare STT to GMAW-P for low-cost automation of out of position GMAW as a competitor to manual GTAW and semi-automatic
GMAW. The research conducted by the author showed mechanized GMAW-P, at 2-4 m/min, to be almost three times more productive than mechanized STT for fillet welding the thin C-276 sheet, and almost nine times more productive than manual GTAW or semi-automatic GMAW. The sponsor was happy since they also made the GMAW-P equipment. This is another practical example of the benefits of GMAW-P as a high-speed welding process, even on sheet material.
Gaps in joints have long been considered a fact of life in the fabrication industry, and welding has a long history as the process that can take care of the poor fit-up,
facilitated by the high skill level of a good manual welder. However, productivity suffers considerably with this approach by deposition of excess weld metal, increased heat input and distortion, over and above the high labor cost for a skilled or semi-skilled manual welder, and the limited ability of a human operator to weld at high speeds. The original wave of robotic welding was aimed at replacing the welder and lowering the fabrication cost, but in many cases the gap variation was too large for the application of robotics to work satisfactorily.
The author has seen robotic welding operations where a manual welder has
programmed a robot to weave over a large gap producing a large weld size with high heat input and distortion. This was in an automotive Tier 2/Tier 3 supplier producing welded cross-car dashboard beams. The brackets were produced in-house where the stamping tolerances were in direct control of the same company. Rather than alter the stamping to produce a well fitting part, the large gap created by poor fit-up was being bridged by welding, causing the whole assembly to fail to meet final inspection tolerances because of significant bending distortion around this high heat input weld. This is a rather extreme example, but one drawn from first-hand experience in working directly with the supplier to help them identify the source of the problem.
Modern arc welding robots are equipped with through the arc (TTA) seam tracking to cope with gap variation and seam following. However, to maximize productivity the whole fabrication process has to be considered from first-operations such as cutting and bending, through stamping and other forming operations such that good fit-up is achieved. If this is ignored, the welding process, even though it may be robotic, has to slow down to cope with gap-bridging and avoid burn-through on thinner materials.
Part of the issue is that the productivity, of a welding process is relatively poorly understood and thus a hidden cost in many ways. The usual argument is that it is ‘too expensive’ to improve fit-up, when springback from a forming operation, or poor fit from a stamping operation leaves the welding operation to cope with large gaps. In this case the context of large is a gap of more than 0.5 T where T is the material thickness.
1.1.1 Dispelling the Myths about GMAW-P
There have been over 250 articles and papers published on the subject of GMAW-P, and numerous theses for higher degrees. Despite this, the myths persist, perhaps because of the sometimes highly technical nature in which the wide array of possibilities offered by GMAW-P parameter settings have been studied, including metal droplet transfer, synergic logic controls, and algorithms for pulse parameter development. These subjects are usually presented by the technical community to the technical community. While there have been numerous good general articles on the subject over the years, much of the published work may not have been read by the welding community and welders at large, either because it is presented in specialized journals, or not widely published as is the case with many thesis dissertations or consortia projects. For example, the author ran a 2½ year study of synergic pulsed GMAW in the late 1980s, but this was a confidential consortia project. While the results would in themselves address many of the myths described below, they were not available for widespread publication.
GMAW-P was initially developed in the mid 1960s, to exploit the benefits of high arc stability and low spatter offered by the spray mode of metal transfer at wire feed speeds (WFS) and welding currents below the spray transition point for steel wires; for example, below 230A for a 1.2-mm-diameter wire in Ar-CO2shielding gases. The generation of power supplies available at that time relied on the manual setting and balancing of pulse parameters, namely the pulse current, pulse time or duration, background current, and background time. While this setup could produce good results, it had two major disadvantages. Firstly, the welder had to understand the interactive nature of the individual pulse parameters to obtain stable transfer for a particular wire speed, and secondly, had to reset the pulse parameters for each WFS selected to maintain stable wire burn-off characteristics.
These major drawbacks led directly to the development of synergic pulsed GMAW, although commercial power sources were not produced in significant quantities until the early 1980s, largely because the more sophisticated power electronic devices required were not initially available, and were too costly for widespread application until the 1980s. The invention and continued development of the inverter power source has been crucial to the development and widespread application of GMAW-P.
In GMAW-P the individual pulse parameters are automatically selected from a set of preprogrammed parameters through solid-state electronic logic controls. The use of such controls effectively allows a welder to dial up a current or WFS, and the power source automatically selects the appropriate pulse current and time parameters and the pulse frequency required to burn off the wire at whatever WFS is demanded,
maintaining a stable spray transfer, with concomitant benefits for control of metal transfer at negligible spatter levels.
1.1.2 The Common Myths
There are a wide variety of myths which have been created over the past 15 to 20 years concerning the application of GMAW-P. Some of the more common ones are listed below and explained:
Myth 1 –GMAW-P prevents spatter, and is a spatter-free process
Myth 2 –GMAW-P is a lower heat input process than conventional constant voltage (CV) GMAW
Myth 3 –GMAW-P was invented to weld sheet metal and is more tolerant to burnthrough
Myth 4 –A true square wave pulse is better than other pulse shapes
Myth 5 –GMAW-P is appropriate for all problems with GMAW, in as much as it is better at any WFS than conventional CV GMAW.
Myth 6 –GMAW-P is a slower process than conventional GMAW in terms of welding speed
Many of these myths have become established in industry, often encouraged by the overselling of the equipment as a panacea for all problems. The myths persist and are still promulgated.
1.1.3 Dispelling the Myths
The individual myths are in no particular order, but will be dealt with in the order they are presented above.
Myth 1 – GMAW-P Prevents Spatter, and is a Spatter-Free Process
Unfortunately, the physical nature of the GMAW process, and particularly the way it starts by short circuiting the wire to the workpiece, means that for all practical purposes there will always be some spatter at the start of the weld as the arc is established. This has long been an area of active study, and still awaits a low-cost, robust solution suitable for industrial application. Once in steady-state operation the electronic pulsed control of metal droplet transfer produces a welding condition, which if the torch is manipulated correctly can produce a weld bead which is effectively free from adherent spatter in the vicinity of the joint. In practical terms, GMAW-P offers low spatter operation, which improves weld cosmetic appearance and reduces problems of part fit-up, through spatter deposited on fixturing, in increasingly mechanized and automated welding operations.
However, despite the pulsed current, the arc voltage also needs to be suitable for spray transfer. If the arc voltage is tuned too low, say below 20V, short circuiting may
occur, or the arc action on a larger weld pool may cause metal to be ejected from the pool in the form of spatter. It should be noted that with the wide variety of electronic controls now available, it is also possible to use synergic control for SC transfer, and variants are available such as Lincoln Electric’s STT which electronically senses SC droplet detachment to minimize spatter in a SC operating mode.
Myth 2 – GMAW-P is a Lower Heat Input Process than Conventional CV GMAW
The myth states that using discrete current pulses better controls and lowers the heat input to the weld. While may be true for pulsed gas tungsten arc welding (GTAW) where low pulse frequencies, typically 2 to 10 Hz, used in, it is largely a myth with P-GMAW where pulse frequencies are typically 100 to 500 Hz. Pulsing certainly gives much more control over metal transfer, especially compared to conventional short circuiting or globular transfer in CV GMAW of ferritic steels and stainless steels. However, as far as the weld pool is concerned, and the heat flow into the adjacent metal, the heat input of P-GMAW is effectively no different to that of conventional GMAW for the same current and voltage.
Myth 3 – GMAW-P was Invented to Weld Sheet Metal and is More Tolerant to Burnthrough
The GMAW-P process was invented to achieve the best control of metal transfer across the entire range of useable WFS for each particular diameter. This is because spray provides the most arc stability and thus the best opportunity to transfer metal across the arc and deposit it where it is desired. Thus, the development of GMAW-P was aimed as a broad range of material thicknesses, not just sheet metal. Applications range from welding of automotive vehicle frames through welding of circumferential pipe joints. In fact, with the open arc and consequently higher arc voltage, GMAW-P is somewhat less suited to sheet metal applications than controlled short circuit welding, although it can be used with careful control of arc voltage in semiautomatic mode. Mechanized welding of sheet metal, where the travel speed (TS) can be considerably higher is very attractive. A project at EWI (Harris, 1998) demonstrated that GMAW-P could be used to weld lap-fillet joints at 2.8 m/min on Ni alloy C-276 in the 3F vertical down position and 2F H-V fillet welds were made at 2.0 m/min. Welds were free from spatter and had a pleasing slightly convex weld profile desirable for the application. The Ni alloy weld pool is thought to be more viscous than that for other alloy systems, and thus is considered less prone to humping defects.
Myth 4 – A True Square Wave Pulse is Better than Other Pulse Shapes A true square waveform is only really produced with expensive transistor power sources. Almost all commercial GMAW-P power sources contain some inductance in the circuit resulting in some minimal delay in current rise at the start of the pulse. Many power supplies are now inverter designs which can have an inherent current ripple on the peak and background current waveform associated with the switching frequency of the inverter.
As part of a large group-sponsored project on GMAW-P a study of five power source control designs and waveform shapes for GMAW-P with various pulse shapes
determined that there was negligible difference between the performance of each in terms of the effect on weld penetration for the same welding parameters and thus welding power. The important criterion is that enough energy is supplied in the pulse to detach a droplet. Typically the droplet is approximately the size of the wire
diameter. For this case, for similar welding power, the results of a variety of
waveform shapes are essentially the same in terms of weld bead characteristics such as bead width and penetration depth.
Myth 5 – GMAW-P is Appropriate for all Problems with GMAW, Since it is Better at Any WFS than Conventional CV GMAW
No welding process is a panacea for all welding problems. Each process has niche areas where it can be used more effectively than other processes. The GMAW process is the most widely industrially applied process of any welding process, arc or resistance. In many instances conventional GMAW does an adequate job. However, with ever increasing focus on weld quality and industrial competitiveness, the
GMAW-P process should be examined to see whether it can enhance weld quality through spatter reduction, weld profile control, and overall consistency of operation. Results achieved using spray transfer with conventional GMAW will be hard to beat. The GMAW-P technique provides the ability to use the advantages of spray transfer at WFS where SC or globular transfer would otherwise be the options with lower WFS using conventional GMAW.
One of the more important attributes of GMAW-P is that it allows spray transfer to be used out of position. This opens up a number of possibilities, including welding of pipe joints in the 5G and 6G fixed positions.
Myth 6 – GMAW-P is a Slower Process than Conventional GMAW in Terms of Welding Speed
This myth may have come from a parallel drawn from pulsed GTAW where TS needs to be sequenced with pulse frequency to get the required overlap and weld ripple pattern. With GMAW-P the pulse frequency is in the range of 100 to 500Hz, rather than the typical 2 to 10 Hz used for pulsed GTAW, so there is no need to weld slowly. There is no technical justification for supposing that GMAW-P should be slower that conventional GMAW for the same wire feed speed. As mentioned earlier a recent project at EWI demonstrated that GMAW-P could be used to weld lap-fillet joints at 3.75 m/min on Ni alloy C-276 in the vertical down position. This is a very high welding speed, and suitably indicates the potential for high welding speeds with GMAW-P.
1.1.4 The Good News
While the myths persist, many users have found GMAW-P to be a very effective tool, and the use of this variant of GMAW has found widespread applications from
welding of sheet metal through welding pressure vessel steels. The level of
sophistication of the power sources available today is daunting to some, but for the end user, should be viewed as offering a wider array of possibilities and flexibility
than ever before. While most applications reflect the general usage of materials, i.e., ferritic steels, stainless steels, and Al alloys in that order, the process is very suitable for welding Ni alloys, Cu alloys, and even Ti alloys. For the majority of applications and users the preprogrammed parameters for steel, stainless steel, and Al alloys for various wire sizes and shielding gases are sufficient for most needs. These are set up as simple toggle switches on most power supplies, leaving the welder to simply set the WFS (or current control depending on the labeling of the main control knob) and trim the arc voltage (usually5 to 10% of a preprogrammed voltage). The
possibilities for user pulse programming and parameter storage, where needed, are now wider than ever. The current state of developments in solid-state electronics and inverter power sources, has yielded systems such as Lincoln Electric’s Wave Designer software which allow almost infinite control of pulse parameters and power source characteristics. Obviously, these sophisticated controls are not for the uninitiated, but with suitable control by qualified personnel, they are very powerful tools. GMAW-P equipment has offered conventional CV GMAW from the earliest days along with preprogrammed parameters for common combinations of wire type, wire diameter, and shielding gas. The most sophisticated power supplies obviously also offer these more conventional operation modes.
For sheet metal applications the following are typical;
Almost all welds are single pass and the majority are lap welds Acceptable quality and high productivity are the key requirements Weld sizing is not well defined, especially for welding of sheet metal Minimizing joint gaps is key to maintaining high welding productivity
Most data is based on single torch GMAW in either short-circuit (SC) mode or using GMAW with direct current (DC) or GMAW-P
Weld humping limits travel speed and thus welding productivity for high-speed welds
The maximum potential travel speed to make welds with single torch GMAW-P needs to be evaluated to establish a baseline from which to compare other processes. The limiting effect of joint gaps on maximum travel speed is part of this baseline.
To make significant strides in welding productivity, joint-fit up is a critical
requirement rather than a preferable thing if the potential productivity and welding speed improvements offered by hybrid LBW/GMAW-P are to be realized. As such, this process needs to be studied with joint fit-up set at a minimum.
To overcome the problems with productivity from the perspective of the welding process, the primary need is suppressing the weld humping defect to increase the travel speed at which acceptable welds can be obtained. To achieve this, the humping defect needs to be studied as well as welding processes and techniques that can more readily produce a small fillet weld size. The associated research objective is thus to conduct a
fundamental study of the humping phenomenon and its mechanisms to understand how to suppress or eliminate it while welding at high travel speed.
2.0 LITERATURE REVIEW AND INDUSTRY SURVEYAlmost 200 papers and articles relevant to the overall subject matters have been reviewed: high-speed GMAW, GMAW-P, GMAW-VP, laser, laser/GMAW hybrid welding, weld pool dynamics and humping, and weld pool modeling. Many of these are cited in this literature review.
2.1 Process Studies and Welding Productivity
GMAW using SC or pulse spray transfer are the preferred methods used by industry for welding light structures because of their lower heat inputs.
The arc welding equipment industry has been busy producing a wide new array of GMAW variants, including twin-wire GMAW, GMAW-VP, STT GMAW, and GMAW-MP in addition to enhanced CV GMAW, and GMAW-P equipment of increasing reliability, stability, and hence weld quality and consistency. The newer GMAW variants and some of their application areas are discussed below.
In a scenario of continuous improvement and cost reduction, welding productivity increases through robotics and automation have and will continue to be achieved. The development of newer welding techniques and processes is often aimed at higher productivity through the use of higher welding speeds and thus deposition rates. A big impediment to welding productivity is the tendency to over-weld small fillet welds in thin plate and sheet products. Over-welding results in higher welding costs, including additional welding power, electrode wire, higher distortion (and distortion correction costs), and lost productivity. Two processes that are relatively new are TGMAW and laser/hybrid GMAW. Both offer the flexibility to apply to plate products and thicker sheet products, with limits generally accepted to be around 1.6-mm thickness at the lower end.
The productivity of GMAW, GMAW-VP, GMAW-P, TGMAW, and LBW/GMAW hybrid processes are reviewed here as a context and benchmark for the present research. Arc welding processes use electrical energy to melt or fuse metals to produce a joint between two or more parts. All processes are characterized by an electrical arc between an electrode and the workpieces. These processes, their advantages and disadvantages, and their applications for welding sheet products are described in the following sections.
2.2 Gas Metal Arc Welding
The GMAW process (also known as MIG or MAG welding) is characterized by the fact that an arc is formed between the end of a continuous spool of electrode wire and the workpiece, Figure 2.1. The solid wire is continuously fed through a contact tip in the torch, and melts to form the weld bead joining the base metals. The wire feed rate is balanced to the burnoff rate to maintain a stable arc. The wire type is selected to give the weld metal a matching (but often overmatching) strength compared to the base metal. The weld area around the arc is protected by a shielding gas supplied from the torch.
Figure 2.1 GMAW Process
GMAW weldments can be made in all positions, especially using pulsed-current, GMAW-P, thus the process is ideally suited to automation, especially through arc welding robots. Gap tolerance for GMAW is good, with joint gaps up to 1T being tolerable.
The welding parameters that must be controlled to produce acceptable welds include welding current, arc voltage, WFS, torch TS, torch travel and work angles, and shielding gas flow rate. The joint gap should be minimized to achieve the best joint quality and productivity.
The major advantages of the GMAW process are its high productivity and reliability coupled with low cost. The process is suited for automation, and very little cleanup is required after welding. The equipment can be deployed on welding robots with relative ease, and single-side access only is required. In addition, the process is suitable for many different alloys, including carbon and low alloy steels, stainless steels, Al alloys, Ni alloys, Cu alloys, and Mg alloys.
The disadvantages of GMAW are that plant ventilation is required to remove welding fumes, and that protection is needed from strong drafts to avoid loss of shielding gas efficiency which can lead to porosity. Welding of coated steels can cause porosity by volatilization of zinc-rich coatings. This can be mitigated by correct development and implementation of welding procedures.
The GMAW process already has widespread usage in the automotive supplier network, ranging from SUV and light truck frames to exhaust, catalytic converter, seat frames, suspensions, and engine cradles. GMAW is widely used in structural applications for making fillet welds on lap, corner and T-joints, and also in light industrial applications. The process is widely applied using manual, mechanized, and robotic techniques. Consumable electrodes can be solid or metal-cored and used in a variety of metal transfer modes: SC, globular, and spray. Cu-based electrodes are
used for braze welding cast iron and galvanized sheet. Conventional CV power supplies are very affordable.
2.2.1 GMAW Including GMAW-P
As a long-established process, GMAW, and in the last 20-25 years, GMAW-P, have rightly developed a standing atop the most widely used and flexible production welding processes, both in terms of application across a broad range of materials, but especially in terms of flexibility for deployment with a wide array of mechanization and automation. Application experience and production robustness is broadest at relatively modest TS, often stated to be in the 0.5-1.0-m/min range
The GMAW-P process has been widely reviewed before, and the benefits are considered to be well understood in the automotive supplier network, especially among the Tier 1 suppliers. Current pulsing has the benefit that spray transfer can be achieved across the entire range of WFS, maintaining the most stable arc conditions, which relate directly to weld quality, consistency, and very low spatter levels. Attached to a modern six axis welding robot, or other mechanized welding system, this provides a very flexible manufacturing tool. GMAW-P has been heavily used since the late 1980s by automotive suppliers such Tower Automotive which had several hundred machines in production welding operations at that time for welding light truck frames and other parts. Almost all applications until fairly recently were for steel. In the last several years GMAW-P of Al alloys has become of increasing interest and application, especially for components such as suspension parts and engine cradles. For example, the Audi A8 spaceframe is welded predominantly with GMAW-P.
Metal-cored wires offer another dimension for high-quality and high-productivity GMAW whether by GMAW-P or conventional CV GMAW. The metal powder in the wire core offers enhanced deposition rates and welding speeds compared to typical solid wire GMAW. The cored nature of the consumable also offers a cheaper production route for alloyed wires such as the Type 409 wires for welding Type 409 exhaust components, which can be Ti, Nb, or Nb/Ti stabilized for grain size control and enhanced mechanical properties of weldments.
GMAW-P is widely used on applications that compete with SC welding (light gauge) and spray for out-of-position welding. Waveform development tools (software), servo-wire feeders, and real-time parameter monitoring may be provided with these advanced systems. Cost is typically two to four times that of CV equipment.
The GMAW and GMAW-P processes have been very widely studied with attention more often in the realms of optimization for productivity along with production robustness. Various well-known generalized optimization methods such as Taguchi, design of experiment (DOE), and other techniques have been applied to welding.
Successful strategies such as ‘Sloping Weld Area Testing’ (SWAT) (Green, 2001), ‘Arcwise’ (Harwig, 2000), and others have been applied that are more directly tailored by and for arc welding research and development. SWAT was carried out using steel and Si bronze consumables for welding steel sheet and tubes simulating joints anticipated for tubular construction of automotive frames (Green, 2001). This